In our experiments, a series of electron-only devices were fabricated for studying the effect of electron injection and electrical characteristics. The electron-only device structure was ITO/Alq3 (80 nm)/n-doped ETL (10 nm)/Al (150 nm), in which the doping concentration of CsF in MADN are 0%, 10%, 20% and 30%, respectively.
Figure 6-19 plots the I-V characteristics of these electron-only devices.
Lower operational voltage and higher current density dependency were observed in CsF doped electron-only device as compared to that of undoped device, which indicate that the electron injection from Al cathode can also be improved by doping CsFinto MADN.
Figure 6-19 I-V characteristics of CsF-doped electron-only devices.
To understand the electrical doping phenomena, the electron-only devices are further investigated by AS as shown in Figure 6-20. As we discussed in the PAK2 case (Section 6.2.1), the low-frequency peaks (G/F peaks at 200-4000 Hz) are assigned to be associated with a single RC time constant of the n-doped MADN layer and high-frequency peaks (G/F peaks at 0.13-0.15 MHz) are associated with a single RC time constant of parasitic series resistance . It is also found that the high-frequency peak is temperature-independent and the low-frequency peak is temperature-dependent. Furthermore, the Ea of n-doped MADN layer can be derived from the slope of relationship between of ln(F) and 1000/T as plotted in Figure 6-21(a), when the doping percentage of CsF was increased from 10%, to 20%, and 30%, the activation energy (Ea) of MADN could be greatly reduced from 0.157 eV to 0.145 eV and then to 0.099 eV. In this case, Ea represents the energy separation between the edge of the LUMO level and Fermi level of MADN as shown in Figure 6-21(b), the decrease of Ea
indicates that the Cs2CO3 incorporation reduces this separation, which lowers the electron injection energy barrier between MADN and Al, thus improves the electron injection from Al cathode to MADN.
Figure 6-20 Temperature-dependent G/F-F spectra at zero bias of electron-only devices with various doping concentration.
Figure 6-21 (a) Characteristic of ln(F) vs 1000/T of CsF-doped devices derived from the low-frequency peaks in Figure 6-20. (b) Schematic energy diagram of Al/n-doped MADN interface.
6.4.2 Device performances of using n-doped layer composed of CsF-doped MADN
As illustrated in Figure 6-22, three following devices are fabricated to test the efficacy of the n-doped ETL composed of MADN doped with CsF. First one is the standard device with conventional structure of ITO ITO/CFx/NPB (60 nm)/Alq3 (75 nm)/LiF (1 nm)/Al (150 nm), second and third are i-i-n devices with structures of ITO/CFx/HTL (60 nm)/Alq3 (65 nm)/MADN: 30% CsF (10 nm)/Al (150 nm), in which NPB and MADN were used as HTL, respectively.
Figure 6-22 Device architecture of standard device and i-i-n devices.
The EL performances are summarized in Table 6-4, it is apparent that i-i-n devices with MADN doped CsF layer can achieve higher efficiency and low drive voltage at 20 mA/cm2. Significantly, inducing the n-doped layer of MADN doped CsF can improve the electron injection from Al cathode, which fully agrees the results of I-V characteristic and AS measurement. These results indicate that MADN can be used as an efficient host for n-type dopant CsF and reduce the drive voltage in OLED devices. Furthermore, the performance of
i-i-n device with MADN as hole transport layer (HTL) can boost up to 6.1 cd/A as shown in Figure 6-23, the enhancement of device performance agrees the result of the utilization of MADN as HTL, which we will discuss in Section 7.3.
Table 6-4 EL performances of OLED devices at 20 mA/cm2.
Figure 6-23 Current efficiency vs current density characteristics of OLED devices.
In this chapter, we study the electrical characteristics and doping effect of
p-doped (WO3-doped MADN) and n-doped (PAK2-doped BPhen and CsF-doped MADN) organic layers by measuring I-V curves and temperature-dependent AS. The results indicate that incorporations of p-type
E. Q. E.
Standard 6.3 3.6 1.8 1.1 (0.36, 0.55)
i-i-n (NPB) 5.2 3.3 2.0 1.1 (0.36, 0.55)
i-i-n (MADN) 5.5 6.1 3.5 1.9 (0.38, 0.55)
(WO3) and n-type (PAK2 and CsF) dopants can reduce the activation energy, which represents the energy separation of between the Fermi level and the HOMO level for p-type case, the LUMO level for n-type cases, respectively, and can further improve the carrier injection from the electrodes.
On the other hand, the results of PAK2 case also show that potassium metal carboxylates are also useful for n-type doping with an easy and stable evaporation process as compared to inorganic salts. However, the mechanism of thermal deposition of these kind of materials is still not well understood, even we investigated this phenomenon by QCM.
Moreover, the results of MADN cases imply that MADN can be a host for both p-type (WO3) and n-type (CsF) dopants and these p-doped and n-doped MADN layers can effectively applied to OLED devices, which is an useful information for simplifying the OLED device architecture by multifunctionally utilizing MADN, and the further experiments are described in next chapter.
 S. R. Forrest, Chem. Rev. 97, 1793 (19997).
 N. Karl, Defect Control in Semiconductors, Vol. II, North Holland:
 C. W. Tang, Appl. Phys. Lett. 48, 183 (1986).
 C. W. Tang, S. A. Van Slyke, Appl. Phys. Lett. 51, 913 (1987).
 J. Kido, K. Nagai, Y. Okamoto, IEEE Trans. Electron Devices 40, 1342 (1993).
 I. D. Parker, J. Appl. Phys. 75, 1656 (1994).
 T. Wakimoto, Y. Fukuda, K. Nagayama, A. Yokoi, H. Nakada, M. Tsuchida,
IEEE Trans. Electron Devices 44, 1245 (1997).
 E.I. Haskal, A. Curioni, P.F. Seidler, W. Andreoni, Appl. Phys. Lett. 71, 1151 (1997).
 Y. E. Kim, H. Park, J. J. Kim, Appl. Phys. Lett. 69, 599 (1996).
 L. S. Hung, C. W. Tang, M. G. Mason, Appl. Phys. Lett. 70, 152 (1997).
 G. E. Jabbour, Y. Kawabe, S. E. Shaheen, J. F. Wang, M. M. Morrell, B.
Kippelen, N. Peyghambarian, Appl. Phys. Lett. 71, 1762 (1997).
 S. E. Shaheen, G. E. Jabbour, M. M. Morrell, Y. Kawabe, B. Kippelen, N.
Peyghambarian, M. F. Nabor, R. Schlaf, E. A. Mash, N. R. Armstrong, J. Appl.
Phys. 84, 2324 (1998).
 C. H. Lee, Synth. Met. 91, 125 (1997).
 F. Li, H. Tang, J. Anderegg, J. Shinar, Appl. Phys. Lett. 70, 1233 (1997).
 H. Tang, F. Li, J. Shinar, Appl. Phys. Lett. 71, 2560 (1997).
 Y. Park, J. Lee, S. K. Lee, D. Y. Kim, Appl. Phys. Lett. 79, 105 (2001).
 J. Lee, Y. Park, S. K. Lee, E. J. Cho, D. Y. Kim, H. Y. Chu, H. Lee, L. M.
Do, T. Zyung, Appl. Phys. Lett. 80, 3123 (2002).
 J. Liu, A. R. Duggal, J. J. Shiang, C. M. Heller, Appl. Phys. Lett. 85, 837 (2004).
 T. Mori, H. Fujikawa, S. Tokito, Y. Taga, Appl. Phys. Lett. 73, 2763 (1998).
 E. Ettedgui, H. Razafitrimo, Y. Gao, B. R. Hsieh, Appl. Phys. Lett. 67, 2705 (1995).
 J. Yoon, J. J. Kim, T. W. Lee, O. O. Park, Appl. Phys. Lett. 76, 2152 (2000).
 P. He, S. D. Wang, S. T. Lee, L. S. Hung, Appl. Phys. Lett. 82, 3218 (2003).
 C. Ganzorig, M. Fujihira, Jpn. J. Appl. Phys. Part 2 38, L1348 (1999).
 C. Ganzorig, K. Suga, M. Fujihira, Mater. Sci. Eng. B 85, 140 (2001).
 S. H. Kim, J. Jang, J. Y. Lee, Appl. Phys. Lett. 91, 103501 (2007).
 T. Hasegawa, S. Miura, T. Moriyama, T. Kimura, I. Takaya, Y. Osato, H.
Mizutani, Proceedings of SID’04, p. 154, May 23-28 (2004), Seattle, Washington, USA.
 W. Brütting, H. Riel, T. Beierlein, W. Riess, J. Appl. Phys. 89, 1704 (1994).
 S. Odermatt, N. Ketter, B. Witzigmann, Appl. Phys. Lett. 90, 221107 (2007).
 M. Pfeiffer, K. Leo, and N. Karl, J. Appl. Phys. 80, 6880 (1996).
 Y. Matsuda, C. Ganzorig, K. Suga, M. Fujihira, Ext. Abstracts, 50th
Spring Meeting, Jpn. Soc. Appl. Phys. and Related Soc. p. 1404, 27p-A-4 (2003).
 C. Ganzorig, M. Fujihira, Appl. Phys. Lett. 85, 4774 (2004).
 Y. Li, D. Q. Zhang, L. Duan, R. Zhang, L. Duo, Y. Qiu, Appl. Phys. Lett. 90, 012119 (2007).
 G. Z. Sauerbrey, Z. Phys. Chem. (Munich) 155, 206 (1959).
 H. Jiming, L. Lijia, B. Danielsson, X. Zhou, L. Wang, Anal. Chim. Acta 423, 215 (2000).
 A. B. Daniel, D. W. Michael, Chem. Rev. (Washington, D.C.) 92, 1355 (1992).
 B. W. D’Andrade, S. R. Forrest, and A. B. Chwang, Appl. Phys. Lett. 83, 3858 (2003).
 H. Aziz, Z. D. Popovic, N.-X. Hu, A. M. Hor, G. Xu, Science 283, 1900 (1999).
 S. A. Van Slyke, C. H. Chen, C. W. Tang, Appl. Phys. Lett. 69, 2160 (1996).
 C. C. Chang, M. T. Hsieh, J. F. Chen, S. W. Hwang, C. H. Chen, Appl. Phys.
Lett., 89, 253504 (2006).
Organic Light-Emitting Diodes based on one Multifunctional Bipolar Material
Since Tang and Van Slyke developed the multi-layer OLEDs , tremendous efforts have been directed toward improving the device performance and operational lifetime. It was recognized that E. Q. E. of OLEDs depends heavily on the efficiency of carrier injection, transport and recombination as well as the balance of the holes and electrons , however, the mechanism underlying these key performance parameters are not well understood.
The basic OLED device has a bilayer organic thin-film structure such as ITO/NPB/Alq3/LiF/Al, where ITO is the anode, LiF/Al is the cathode, NPB and Alq3 are the HTL and ETL, respectively. During operation, the injected holes and electrons recombine at or near the HTL/ETL interface, producing EL.
However, this typical NPB/Alq3 structure in general does not necessarily provide the configuration to achieve a balanced carrier injection/transportation that leads to recombination. One of the reasons is that the excess holes would accumulate at HTL/ETL interface and generate NPB+ and Alq3
+ radical cations.
It has been suggested that exciton quenching at the NPB/Alq3 interface due to the accumulation of NPB+ radical cations at the interface impacts significantly on the current efficiency [3,4]. Moreover, it has also been reported that Alq3 cationic species would easily be produced when hole carriers exist excessively, resulting in deterioration of device lifetime [5,6,7].
It has been shown that much improved OLED performance can be realized
using a HIL/HTL structure, where HIL is the “hole-injection” layer inserted between the anode and the HTL. For example, with CuPc  as the HIL as in CuPc/NPB/Alq3 where Alq3 also functions as the emissive layer, long-lived OLEDs have been obtained. Another common HIL material is 4,4’,4”-tris[N-(3-methylphenyl)-N-phenylamino] triphenylamine (MTDATA) , with which enhanced current efficiency and operational stability have been demonstrated. High-efficiency OLEDs have also been reported in various HIL/HTL configurations [10,11,12,13,14]. Furthermore, low-voltage and high-efficiency OLEDs can be realized with a p-doped HTL [15,16,17], in which the layer thickness can be readily adjusted for optimal light extraction. It has been suggested that the enhanced performance in HIL/HTL devices is due to a sequence of cascaded hole-injection barriers present in the HIL/HTL/ETL structure, which produces a “balanced” electron-hole recombination at the HTL/ETL interface [18,19].
Consequently, finding a way of reducing the number of holes or increasing the number of electrons reaching the emission layer is considered one of the most direct and economic solutions to improve device efficiency. Recently, it was found that the hole mobility can be efficiently controlled by incorporating the composite hole transporting layer (c-HTL) of NPB: copper phthalocyanin (CuPc) (1:1) to balance the charge carriers  from which the device efficiency can be significantly enhanced. However, the fabrication process is complicated, which requires precise control and in particular, using the environmentally unfriendly CuPc.
In addition to the well-known property of large bandgap and high fluorescence quantum yield, anthracene-based derivatives have been shown to
possess bipolar character and moderate-to-high carrier mobilities. In this chapter, we summarize examples of anthracene-based compounds that have successfully been used as charge transport materials both for hole and electron transport layers, respectively. We also demonstrate the bipolar nature of MADN by studying the electrical characteristics of carrier-only devices and further simplify the OLED device structure by taking the advantage of this bipolar nature.
7.2 Review of anthracene-based materials used in HTL of OLED devices
As early in 2002, Shi and Tang at Kodak had claimed in a US patent in which anthracene-based derivatives were found to be useful as hole transport layer in producing efficient OLED devices . Representative structures are shown in Figure 7-1. In the past, although arylamines have been used extensively as hole transport materials in OLED devices, they do have a number of deficiencies. First, as a class of organic materials, they are relatively strong electron donors, meaning that they can be readily oxidized and may be unstable in ambient environments. Second, when placed adjacent to an ETL as HTL in a OLED device, the arylamines may interact with the strongly accepting electron transport layer to produce non-emissive charge-transfer species which will result in a loss of EL. Third, because of the low ionization potential of the arylamines HTL and the hole-blocking ETL will cause the holes to localize in the arylamines to form the non-emissive amine radical cations which will also lead to quenching. To alleviate the aforementioned shortcomings in HTL, anthracene-based derivatives have been used recently for improving the OLED device performance.
Figure 7-1 Chemical structures of anthracene-based HTLs.
In 2002, Tao et al.  synthesized a series of diaminoanthracene derivatives and used them as hole transport material in a green emitter. The structure of 9,10-bis(2-naphthylphenylamino)anthracene (-NPA) is depicted in Figure 7-1 as well. The
-NPA-based device, with structure of ITO/-NPA (40nm)/Alq3 (50 nm)/Mg:Ag alloy (10:1, 55 nm), achieved an EL efficiency of 7.7 cd/A and 5.4 lm/W with an EL peaking at 530 nm and CIEx,y of (0.31, 0.63). In particular, the device has an extremely low turn-on voltage of 2.6 V without any
p-dopant, suggesting that diaminoanthracene derivatives are excellent for holetransport layer with HOMO of 5.54 eV. After that, there was another patent by Yu et al.  claiming that the introduction of diarylamino groups on 2-/6- positions of anthracene moiety could improve hole transport property considerably and is useful as hole transport layer in OLEDs.
Later, triphenylamine end-capped anthracene derivatives have also been characterized for efficient blue emitter as well as HTL  whose typical structure of 9-Phenyl-10-(4-triphenylamine)anthrancene (PhAA) is also shown in Fig. 7-1. These type of materials show high Tg of 104-162 °C with good
thermal stability, and strong blue emission of quantum yields of 0.44-0.48.
Based on these compounds, efficient deep-blue emissions have been achieved by using a simplified two-layer device architecture of ITO/PhAA (50 nm)/TPBI (30 nm)/LiF/MgAg with maximum efficiency of 3.0 cd/A (2.4 lm/W) and CIEx,y of (0.14, 0.14).
7.3 Using MADN as HTL
In our previous work, MADN has been found to be an efficient blue host material which forms stable thin-film morphology upon thermal evaporation and has a wide energy bandgap . Moreover, the hole mobility of MADN has been measured to be (3-9) × 10-3 cm2/Vs by TOF technique and discussed in
Section 5.3.2, which is even higher than that of common-used hole transportmaterial NPB (5.1 × 10-4 cm2/Vs) , indicating that MADN can be used as a hole-transport material in OLED devices.
In this section, we study the electrical characteristics of I-V dependence and AS of devices in which the conventional HTL, NPB, is replaced with MADN and find that it could simultaneously improve the carrier recombination in the device and significantly enhance the device efficiency and operational lifetime as well.
7.3.1 Admittance measurements of MADN/Alq3
bilayer structureFor studying the transport phenomenon and electrical characteristics, two additional hole-only devices were also fabricated. The structure of hole-only devices were ITO/CFx/MADN (30 nm)/Alq3 (60 nm)/Al (150 nm) and ITO/CFx/NPB (30 nm)/Alq3 (60 nm)/Al (150 nm), respectively. Figure 7-2 shows the I-V characteristics of the hole-only devices. Higher operational voltage and smaller current density dependency were observed in device B with
MADN as compared to that of the device A. For instance, the turn-on voltage of hole-only devices A and B are 2.4 V and 3.0 V, respectively. We attribute the high drive voltage of MADN device to the large energy gap between MADN and ITO anode as compared to those of NPB hole-only device. (The HOMO levels of MADN and NPB are 5.8 eV and 5.4 eV, respectively.) The electrical properties of the hole-only devices are further investigated by temperature-dependent AS.
Figure 7-2 I-V characteristics of hole-only devices.
The fundamental theory of AS are describe in Section 2.10. Figure 7-3(a) plots the temperature-dependent G/F-F spectra measured at zero bias of the hole-only device of MADN, in which shows two distinct G/F peaks which are proportional to the dielectric loss. The loss peak can be described by the classical Debye frequency response which is given by
)2 frequency. It is evident that the high-frequency peak is temperature-independent
and would not shift at different temperature. On the other hand, the low-frequency peak is temperature-dependent, it will shift toward lower frequency region at low temperature. According to the results of PAK2 case (Section 6.2.1), the high-frequency peak (G/F peak at 0.45 MHz) is associated with the RC time constant of parasitic series resistance and the low-frequency loss peaks (G/F peaks at 250-7300 Hz) are assigned to be associated with the single RC time constant of MADN layer. Similar result can be also observed in the hole-only device of NPB as depicted in Figure 7-3(b).
Figure 7-3 Temperature-dependent G/F-F spectra at zero bias of hole-only devices (a) MADN and (b)NPB.
In addition, as the results we discussed in PAK2 case (Section 6.2.1), the Ea
can also be derived from the slope of relationship between of ln(F) and 1000/T as plotted in Figure 7-4(a), in which in the Ea value of MADN is found to be 0.655 eV and is larger than that of NPB (0.238 eV). In this case, Ea represents the energy separation between the edge of HOMO level and Fermi level of MADN as illustrated in Figure 7-4(b), thereby, larger Ea value represents the larger injection barrier for holes from ITO anode to organic layers and also the
amount of holes injected from ITO anode is reduced, which agrees with the results of I-V characteristics of hole-only devices as plotted in Figure 7-2. On the other hand, with the lower-lying HOMO of MADN which creates a small barrier (0.2 eV) for holes at the interface between HOMOs of MADN and Alq3 (5.7 eV), there would be fewer holes accumulated at MADN/Alq3 interface as compared to the NPB/Alq3 interface. Therefore, it is expected that the issues of excess hole carriers mentioned earlier can be circumvented by introducing MADN as HTL in OLED devices.
Figure 7-4 (a) Characteristic of ln(F) vs 1000/T of hole-only devices derived from the low-frequency peaks in Figure 7-3. (b) Schematic energy diagram of ITO/MADN interface.
7.3.2 Device performances of using MADN as HTL
In our experiments, four OLED devices are fabricated to demonstrate the efficacy of utilizing MADN as HTL with following structures, Alq3-based devices A and F: ITO/CFx/HTL (60 nm)/Alq3 (75 nm)/LiF (1 nm)/Al (150 nm);
C545T-doped devices C and G: ITO/CFx/HTL (60 nm)/Alq3: 1% C545T (37.5 nm)/Alq3 (37.5 nm)/LiF (1 nm)/Al (150 nm). For comparison, the HTL of
devices A and C is NPB and the HTL of devices F and G is MADN, respectively.
The detailed EL performances are summarized in Table 7-1. It is noted that the voltage required at a given current density of device with MADN as HTL is higher than that of the standard device, which is in complete agreements with (3.6 cd/A and 13.3 cd/A) as shown in Figure 7-5. Furthermore, the utilization of MADN as HTL would not impact on the emission color, the CIEx,y coordinates are essentially identical to those of the standard devices as summarized in Table 7-1. It can also be observed that the current efficiency of device G is sustained at 21.3 cd/A even at 450 mA/cm2 suffers essentially no current-induced quenching, and there is no color shift with respect to varying drive currents as the CIEx,y